# To determine the specific gravity of cement

Specific gravity is defined as the ratio of the weights of a given volume of material and weight of an equal volume of water.To determine the specific gravity of cement, kerosene which does not react with cement is used.

Apparatus

Weighing balance

Keroscene

The le chatliers flask is made of thin glass having a bulb at the bottom.The capacity of the bulb is nearly 250 ml. The bulb is 7.8 cm  in mean diameter.The stem is graduated in millimeters.The zero graduation is at a distance of 0.8 cm from the top of the bulb.

At 2 cm  from zero,there is another bulb of length 3.5 cm and capacity of 17 ml. At 1 cm from bulb ,the stem is marked with 28 ml and is graduated up to 24 ml.The total capacity of the stem and bulb is 24 ml.The total capacity of the stem and bulb is 24 ml.The total capacity of the stem and bulb is 24 ml.The portion above the 24 ml mark is in the form of a funnel of diameter 5 cm

Procedure

Dry the flask carefully and fill with keroscene or naphtha to a point on the stem between ze

ro  and 1 ml. Record the level of the liquid in the flask as initial reading.Put a weighted quantity of cement into the flask so that level of kerosene rises to about 22 ml mark,care being taken to avoid splashing and to see that cement does not adhere to the sides of the flask above the liquid .

After putting all the cement to the flask ,roll the flask gently in an inclined position to expel air until no further air bubbles rises to the surface of the liquid .Note down the new liquid level as final reading.

Calculations

Weight of cement used, W =       gm